Kolisetty Alloy Castings - India Manufacturers of Alloy Steel Castings and Non Ferrous Castings Ranging 1 Kg to 300 Kgs.
Address: 16 H I.D.A., Balanagar, Hyderabad-37 India Kolisetty Alloy Castings Contact Person : Address : 16-H, Ida, Balanagar , Hyderabad - , Andhra Pradesh (India) Tel : 91-40-40073252/282/55997228/23077489 Fax : 91-40-40073243/23077489/23176026
Mr. Veeraiah Kolisetty 16H, IDA, Balanagar, Rangareddy, Hyderabad, Andhra Pradesh, India Zip: 500037 91-40-40073282 9849017310
Mechanical properties of metals
Stress Strain Shear strength An explanation of yield and deformation
NoteWhilst the materials considered are metals, the concepts of stress, strain, deformation, hardness, brittleness and ductility discussed below apply across the full materials spectrum, including polymers and ceramics.
StressWhen a material is subjected to an external force, it will either totally comply with that force and be pushed away, like a liquid or powder, or it will set up internal forces to oppose those applied from outside. Solid materials generally act rather like a spring when stretched or compressed, the internal forces come into play, as is easily seen when the spring is released. A material subjected to external forces that tend to stretch it is said to be in tension, whereas forces which squeeze the material put it in compression. An important aspect is not so much the size of the force, as how much force is applied per unit of cross-sectional area. The term stress, symbol (Greek letter sigma), is used for the force per unit area, and has the units of pascals (Pa) with 1Pa being one newton per square metre. Because the reference area is so large, it is normally necessary to use high multiples such as the megapascal (MPa = 106 Pa) and gigapascal (GPa = 109 Pa). However, when we bear in mind that, in electronics, the area over which forces are applied is generally very much smaller, it is useful to keep in mind that one MPa is equivalent to a force of 1 newton applied on a square millimetre of area. [back to top]
StrainA material in tension or compression changes in length, and the change in length compared to the original length is referred to as the strain, symbol1 (Greek letter epsilon). Since strain is a ratio of two lengths it has no units and is frequently expressed as a percentage: a strain of 0.005 corresponds to a % change of the original length.1
In some texts you may find (Greek letter eta) used.
Hookes LawAs you know from a spring, if you gradually stretch it, the force needed increases, but the material springs back to its original shape when the force is released. Materials which react in the same way as a spring are said to be elastic. Typically if we measure the extension of different forces and plot the graph of this, we will find that the extension is proportional to the force applied. Materials that obey Hookes Law exhibit a linear relationship between the strain and the applied stress (Figure 1).
Figure 1: Stress-strain graph for an elastic solid
Many metals follow Hookes Law until a certain level of stress has been applied, after which the material will distort more severely. The point at which straight line behaviour ceases is called the limit of proportionality: beyond this the material will not spring back to its original shape, and is said to exhibit some plastic behaviour (Figure 2). The stress at which the material starts to exhibit permanent deformation is called the elastic limit or yield point.
Figure 2: Stress-strain graph for a typical metal
As Figure 2 shows, if the stress is increased beyond the yield point the sample will eventually break. The term (ultimate) tensile strength is used for the maximum value of tensile stress that a material can withstand without breaking, and is calculated at the maximum tensile force divided by the original cross-sectional area.
Note that there may be substantial differences between the stress at the yield point and on breaking for example, one source quotes the ultimate tensile strength for AISI304 stainless steel as 505 MPa, and the yield tensile strength as 215 MPa. For most engineering purposes, metals are regarded as having failed once they have yielded, and are normally loaded at well below the yield point. With some materials, including mild steel, the stress/strain graph shows a noticeable dip beyond the elastic limit, where the strain (the effect of the load) increases without any need to increase the load. The material is said to have yielded, and the point at which this occurs is the yield point. Materials such as aluminium alloys on the other hand dont show a noticeable yield point, and it is usual to specify a proof test. As shown in Figure 3, the 0.2% proof strength is obtained by drawing a line parallel to the straight line part of the graph, but starting at a strain of 0.2%.
Figure 3: Stress-strain graph for an aluminium alloy
Self Assessment QuestionYou are designing a part with a retention clip which has to spring into place after being pressed into position. By making reference to their stress-strain curves, explain why you would expect steel to be a better choice than aluminium for this application. go to solution
Youngs modulusAs you will appreciate from the shapes of Figure 2 and Figure 3, the slope of the stress/strain graph varies with stress, so we generally take only the slope of the initial straight-line portion. The stress/strain ratio is referred to as the modulus of elasticity or Youngs Modulus. The units are those of stress, since strain has no units. Engineering
materials frequently have a modulus of the order of 109Pa, which is usually expressed as GPa. Some approximate figures for typical electronic materials are given in Table 1. Table 1: Tensile strength and Youngs modulus for selected materials material tensile strength MPa modulus of elasticity GPa 304 stainless steel 500 200 copper 270 120 96% alumina 200 340 aluminium 90 70 Sn63 solder 35 30 epoxy resin 40 3 silicone rubber 10 0.003
QuoteStress is what happens to you from outside; strain is what you feel. Engineers should never say that they feel stressed, even if they have reached their yield point!
CompressionThe compressive strength is the maximum compressive stress that a material can withstand without being crushed. Both strengths have the same unit as stress, and are typically millions of Pa. For most engineering materials, Youngs Modulus is the same in compression as in tension.
HardnessHardness is another measure of the ability of a material to be deformed. There are many different tests for this, but all measure the resistance of a material to indentation, applying a known force to a tool of defined radius which is very much harder than the material being tested. Empirical hardness numbers are calculated from measurements of the dimensions of the indentation.
Figure 4: The Rockwell R hardness test
The principle of one of the simpler tests, the Rockwell R2 test, can be seen in Figure 9. A specimen at least inch (6.4 mm) thick is indented by a inch (12.7 mm) diameter steel ball. A small load is applied, the apparatus is zeroed, and then a larger load is applied and removed. After a short time with the preload still applied, the remaining indentation is read from the scale. 2 As with many standard tests, the units used are American! We have kept kgf to help you gauge the magnitude of the force involved: 1 kilogramforce = 9.81N. For metal measurements, there are alternative Rockwell tests, with different test heads and different loads. You will also find Brinell hardness numbers (BHN), derived from a test which uses a 10mm tungsten carbide ball. Brinell testing is sometimes preferred as it covers a wider hardness range than the Rockwell tests. There is unfortunately little correlation between different hardness tests, but there is reasonable correlation between the hardness results and the tensile strength, at least for given families of alloys. Note that the correlation is to tensile strength rather than yield strength, because plastic deformation takes place during the hardness measurement. [back to top]
Shear strengthSubjected to forces which cause it to twist, or one face to slide relative to an opposite face, a material is said to be in shear (Figure 5). Compared to tensile and compressive stress and strain, the shear forces act over an area which is in line with the forces.
Figure 5: Shear stress applied to an object
The force per unit area is referred to as the shear stress, denoted by the symbol (Greek letter tau), where
Its unit is the pascal (Pa), where force is measured in newtons (N) and area in square metres. When shear stress is applied, there will be an angular change in dimension, just as there is a change in length when materials are under tension or compression. Shear strain, denoted by the symbol (Greek letter gamma), is defined by
where the angular deformation, symbol (Greek letter phi) is expressed in radians. The last approximate equality results from the fact that the tangent of a small angle is almost the same as the angle expressed in radians. This is the reason why some texts give the radian as the unit of strain. Both shear strain and angular deformation are ratios, so have no units. However, it is not unusual for shear strain to be quoted in %, as with tensile strain. Shear stresses are most evident where lap joints are fastened together and forces applied to pull them apart, but are also seen when rods are twisted, or laminated boards bent.
The shear strength of a material is the maximum stress that it can withstand in shear before failure occurs. For example, punching, cropping and guillotining all apply shear stresses of more than the maximum shear stress for that material. A